**Journal Name **

## ARTICLE

*a.*

* Department of Condensed Matter Physics, J. Stefan Institute, Jamova 39, SI-1000 *
*Ljubljana, Slovenia *

*b.*

* Jožef Stefa I ter atio al Postgraduate School, SI-1000 Ljubljana, Slovenia *

*c.*

* Diparti e to di Chi ica e Chi ica I dustriale, U iversitá degli studi di Pisa, via *
*Moruzzi 3, 56124 Pisa, Italy *

*d.*

* Institute of Physics, Academy of Sciences of the Czech Republic, Na Slovance 2, *
*182 21 Prague 8, Czech Republic *

Received 00th January 20xx, Accepted 00th January 20xx

DOI: 10.1039/x0xx00000x

**www.rsc.org/ **

**Mesogen vs. crosslinker resolved molecular order and **

**reorientational exchange using deuteron NMR **

J. Milaveca,b, V. Domenicic, B. Zupa čiča, A. Rešetiča,b, A. Bubnovd, B. Zalara,b

Differences in the temperature behaviour of orientational ordering of structurally equivalent side-chain liquid single crystal elastomers (LSCEs), 2H-labelled in the crosslinker and mesogen, have been studied by deuteron quadrupole-perturbed NMR. The impact of nematic director reorientations on the deuteron NMR spectral shapes was analyzed in terms of discrete reorientational exchange model. This provided for the determination of the degree of domain or nematic director alignment and for the quantification of the influence of the reorientational exchange on the 2H NMR spectra in terms of two parameters, the nematic director orientational dispersion parameter 𝜎 a d the otio al effe ti e ess pa a ete α, respectively. Comparative analysis of model simulations and experimental spectra reveals that mesogenic molecules in oriented LCEs exhibit faster reorientational dynamics as compared to crosslinker molecules and that mesogens and crosslinkers exhibit similar and rather substantial static director orientational disorder.

**Introduction **

Liquid crystal elastomers (LCEs) are materials in which orientational order of conventional liquid crystals is combined

with the elasticity of polymer networks1–3. Many interesting

properties are expected to emanate from the coupling between nematic liquid crystalline order and elastic deformation, among them the giant thermomechanical

response4. One of the most exciting features of these materials

is their macroscopic form changes as a result of the order-disorder transition of the mesogen. A desired unidirectional alignment of domains in the sample can be achieved by

mechanical stretching during the preparation,5 leading to the

so called liquid single crystal elastomers (LSCEs). LCEs are shape-memory materials, due to the ability to memorize the

macroscopic shape under specific conditions6. With increasing

temperature, monodomain LSCEs exhibit a mechanical deformation, specifically a thermomechanical contraction, related to disordering and thermal motion of mesogenic

molecules, attached to the polymer backbone1,7. They are very

good candidates for different technological applications, such as artificial muscles, smart surfaces, microelectromechanical

systems (MEMS), and nanoelectromechanical systems

(NEMS)8–11.

2

H NMR spectroscopy revealed to be very useful to investigate

local molecular orientational behavior of these interesting

materials4,12–15. LSCEs are multicomponent systems, consisting

of a polymer backbone and one or several different types of crosslinking moieties and mesogens. It is anticipated that individual components exhibit different orientational ordering

and segmental dynamics. In previous researches4,12,15, this

aspect of LSCE systems has never been addressed in a greater detail. Specifically, no comparative studies targeted towards elucidating possible differences in the ordering of crosslinker vs. the ordering and dynamical behavior of mesogen have been performed so far. For this reason, we are reporting a systematic study on a series of conventional and newly synthesized siloxane-based side-chain liquid single crystals elastomers (LSCEs) by developing a new, component-resolved NMR methodology.

The molecular dynamics influences the NMR spectra. Typical molecular motions are: (i) high-frequency reorientations of the molecule about its long axis and rotational diffusion of the long molecular axis; (ii) reorientations of the nematic director, equivalently time-averaged direction of the long molecular axis, with an intermediate timescale; (iii) reorientations

mediated by translational displacements (RMTD) mechanism16

with a rather long timescale set by molecular translational diffusion in an environment with spatially inhomogeneous

nematic director17,18.In general, three characteristic motional

narrowing regimes exist, depending on the timescale of molecular dynamical processes, that impact the relation between deuteron quadrupole-perturbed NMR frequency and molecular orientational or conformational state. The particular motional averaging regime is determined by the ratio between the igid latti e spe t al li e width (corresponding to the

inhomogeneously broadened spectrum of a 2H-labelled

molecule with many orientational and conformational states)

*This is the submitted version of an article published in Physical chemistry *

and the characteristic frequency, i.e. the inverse timescale, of the dynamic process providing for reorientational exchange among these instantaneous states.

I the fast otio egi e , he the otio ’s ha a te isti

correlation time is short, typically c <10

-7

s, motional narrowing sets in and the inhomogeneous spectrum is completely averaged-out into a homogeneously broadened spectral line with a Lorentzian line shape. Its line width (fwhm) is related to the spin-spin, equivalently transversal, relaxation

*time T2* via

17

ℎ ℎ𝑜𝑚=_{𝜋𝑇}. (1)

This is a situation encountered with liquid crystals at high
temperatures, in the isotropic state, where a single line is
*found at the Larmor frequency, since S=0. With decreasing *

temperature, reorientational motions are slowed-down, 𝜏_{𝑐}

*increases and, consequently, T2* becomes shorter, resulting in

*increasing fwhmhom* with decreasing temperature. For even

slower molecular motion, with the characteristic correlation

time in the intermediate range (typically 10-7 s c 10

-3

s), motional narrowing becomes incomplete, the spectral lines become non-Lorentzian, and the transversal relaxation

*becomes non-exponential. The total line width and fwhmhom*

do not match anymore since in this intermediate regime, the spectral lines are only partially averaged out. In the slow

motion regime (c

-3

s), the molecular motions are too slow to affect the NMR line shape and there are no motional averaging effects. This is why at low temperatures, e.g. in the crystal phase of a liquid crystal elastomer, the spectrum is inhomogeneously broadened and reflects the distribution of instantaneous molecular orientational and conformational

states, i.e. the igid latti e state of the s ste 18,19

. Specifically, if this distribution is isotropic, a Pake-pattern

spectral shape is obtained in the rigid lattice limit20.

The impact of various molecular dynamics processes is best

estimated by considering the shift of the 2H

quadrupole-perturbed NMR absorption line doublet (± sign)

as a function of parameters , , and :

𝜈±_{= ± 𝜈} _{= ± 𝜈̅} _{(2) }

Here Q is the quadrupole frequency of the deuteron in a C-D

bond, typically 180 kHz21*, the P2* terms are the respective

second Legendre Polynomials of the angle between the director of the nematic phase and the magnetic field, and of

the angle between the C-D bond and the molecular main

axis. Specifically, ≈ ° for the planar hexagonal geometry

of the C-D bond in the case of phenyl ring deuteration. The

respective effective quadrupole frequency is 𝜈̅̅̅̅ ≈ kHz. S is

the nematic order parameter.

Both 𝜈̅ and are averages, the former over fluctuating values

of (for the case of phenyl ring deuteration) and the latter over reorientational fluctuations of the long molecular axis. The inverse characteristic times of these two processes are much shorter than the width of inhomogeneous frequency

distribution 𝛿𝜈 ≈ ⁄ 𝜈 ≈ ⁄ ∙ 8 kHz scanned by the ∙

reorienting and conforming molecule in the course of time. It is thus plausible to assume that, with respect to both

processes, 2H quadrupole-perturbed NMR probes the system

in the complete motional narrowing limit. Nevertheless, below
the nematic-isotropic transition temperature, although still
fast enough for strong motional narrowing, molecular
reorientations are biased (non isotropic), a situation described
*by S0 that leads to onset of doublet splitting (Eq. (2)). *
Dynamical processes may also exist in LSCEs, which modulate

and on much longer timescales, e.g. the RMTD

process. In a network with statically misaligned domains and no interdomain mesogen exchange, the spectrum exhibits inhomogeneous broadening, reflecting the distribution of

directors through the term of Eq. (2). However, in

the case when either (i) the mesogen molecule performs translational diffusion across domains with misaligned directors, or (ii) the domain director fluctuates in time, partial or complete motional averaging of the spectrum is observed.

**Experimental **

**Materials and methods**

**2**

**H quadrupole-perturbed NMR spectroscopy. ** 2H NMR
experiments were carried out with a Bruker Advance III 500
MHz high-resolution solid-state NMR spectrometer, equipped
with an 11.74 T Bruker Ultrashield superconducting magnet, at
a Larmor frequency of 76.753 MHz for deuteron. Spectra were
recorded as a function of temperature by applying the

*quadrupolar echo sequence (90x - ** - 90y- * - ACQ ith a 9 °

pulse of 3.8 *μs. The echo delay * was fixed to 10 *μs and the *

delay between consecutive acquisitions was 28 ms. Measurements were performed on a strip-like sample of about

4 mm × 8,5 mm area. In our geometry, the long edge of the

sample, the nematic director (oriented along the long edge),

and spectrometer field were all pointing vertically.

Temperature was controlled to within 0.1 K accuracy. Thermal equilibration of the sample took about 1000 s at each temperature. Lorentzian line fitting was employed to quantitatively determine the line widths of the spectral lines.

*Transverse relaxation time T2* was measured by applying 2D

pulse programme with solid-e ho se ue e 9 ° - 𝜏 - 9 ° - 𝜏 -

ACQ) and EXORCYCLE22 phase cycling, in the temperature

range between 370K and 300K. The variable time delay 𝜏

ranged from 10 s to 20 ms (10 values) and 1024 - 20480 scans

*have been acquired for each spectrum. T2* values were

determined by fitting the experimental integrals of the

quadrupole-perturbed 2H spectrum as a function of 𝜏 by using

exponential decay function.

**Preparation of Liquid Single Crystal Elastomers. Several **

monodomain LSCE samples were made by thermal

polymerization followed by the two step crosslinking

Fi kel a p o edu e 5

. A pre-polymerization mixture was

prepared by adding the poly(methylhydrosilane), the

crosslinker V1 (15 % mmol units), the mesogen M4 (33,6 % mmol units ) and the mesogen M11 (51,5% mmol units) (see

Scheme 1) to a 2.2 ml of anhydrous toluene. 30 l of

commercial platinum catalyst (COD from Wacker Chemie) was added to the final mixture. In a single sample, only one of the

components was used in a deuterated version, which allowed

for selective 2H NMR measurements. Preparation of V1, M4,

M11 and their deuterated homologues is reported

elsewhere23,24. The prepared mixture was inserted in a circular

reactor inside a temperature-controllable centrifuge. A rate of 5500 rpm (revolutions per minute) and a temperature of 343 K were set for 1 h in order to obtain, in the first step, a partially crosslinked elastomeric network in the form of a film (dimensions 15 mm x 215 mm and thickness of about 0.3 mm). The second crosslinking step consisted of a slow removal of the solvent, accompanied by continual increase of mechanical load (by adding weights) at room temperature. Finally, the sample was dried for 3 days at 343 K and at constant mechanical load.

(a)

(b) (c)

**Scheme 1. Moieties used to prepare the LSCEs: (a) mesogen M4, (b) **

mesogen M11 and (c) crosslinker V1. X=2_{H in deuterated compounds. }

**Results and discussion **

**Director reorientation mechanism and domain misalignment. **

To estimate which motion regime should be assigned to our

spectra of monodomain LSCE 2H-labelled on mesogen or

crosslinker molecules, the homogeneous line width and total line width of spectral lines are compared (Fig. 1). In LSCEs with

2

H-labelled mesogen, the matching between the

*homogeneous line width fwhmhom* in the nematic phase and

the total line width of the spectral line is higher if compared

with 2H crosslinker-labelled LSCEs. This suggests that, assuming

imperfect domain alignment, director reorientations are mechanism is more effective in the case of mesogen molecules than in the case of crosslinker molecules, confirming the scenario of less restricted reorientational dynamics for the case of mesogen.

In the paranematic phase, one can observe an almost complete matching between homogeneous and total line

width for 2H mesogen-labelled LSCEs. Higher temperature

results in a faster translation diffusion and therefore the averaging is more effective, while the variations of order parameter are small.

(a) (b)

**Figure 1. Comparison of homogenous line width (as calculated from **

the T2 measurements) and total linewidth for LSCEs 2H-labelled on (a) mesogen and (b) crosslinker.

In the following, we will analyse the impact of the director

reorientation process on the shape of 2H NMR spectra in the

framework of a discrete reorientational exchange model, in order to obtain more detailed information on the degree of domain alignment, particularly in view of its temperature dependence. We shall demonstrate that domain misalignment and RMTD-like director reorientation in LSCEs can well be quantified by only two parameters, the domain order

parameter _{a} and the characteristic order parameter decay

time Q.

**Theoretical Calculations **

**Distribution of domain directors. In oriented LSCEs, the **

distribution of orientations of domain director, _{𝑎} , 𝜎 , is

assumed to be spherical Gaussian:

stat , 𝜎 = ⅇ

− − tg σ𝜃

ⅇ− tg 𝜎𝜃√ 𝜋 e fi(tg 𝜎𝜃_{√} )tg 𝜎𝜃

. (3)

Here = os [− , ], with denoting the orientation of a

given domain, whereas 𝜎 represents the width of the

distribution. erfi is the imaginary error function. By introducing t 𝜎 = 𝜎 one can rewrite

stat , 𝜎 = 𝑒

− −_{ 𝜎}

𝑒− 𝜎 _{√ 𝜋𝜎 ⅇ fi }
√ 𝜎

. (4)

stat = / is constant for isotropic distribution of

domains, a situation present in polydomain samples. In the above relations we assumed cylindrical symmetry of domain misalignments.

The domain orientational order parameter _{a} ≡ ̅̅̅̅̅̅̅̅̅̅̅̅̅

can be expressed as

a 𝜎 = ∫− a , 𝜎 − ⅆ = − − 𝜎 +

𝑒𝜎

√ 𝜋 e fi_{√} 𝜎 (5)

and the static second moment as

, a 𝜎 = ∫_{−} a , 𝜎 − ⅆ = − 𝜎 +

𝑒𝜎 √𝜋𝜎

e fi

√ 𝜎

. (6)

**Transversal precession of magnetization in the case of **
**reorienting nematic director. The Bloch equation for the **

external magnetic field, with nematic director subject to RMTD or RMTD-equivalent director reorientation process, is

expressed as17,19,25*: *

𝜕

𝜕 = 𝑖 𝜋𝜈± −𝑇 + 𝐷 , (7)

where the extra term 𝐷 represents the contribution of the

*diffusion to the rate of change of the magnetization, and T2* the

spin-spin (transverse) relaxation rate of the magnetization. In the following, we will solve the differential Eq. (7) in a

discrete approximation18. For arbitrary distribution

stat , 𝜎 , e i t odu e a e isop o a ilit a ia le

, 𝜎 with respect to which the probability density

𝑎 , 𝜎 is constant:
, 𝜎 = ∫ ,_{,}
− 𝜎 ,= +
e fi
√ 𝜎
e fi _{√ 𝜎} . (8)

The isoprobability variable [ , ] is introduced in order to

simplify the calculation, specifically to allow for the use of a

relatively simple form of discrete exchange matrix K18,

assuming that, in the equilibrium, all the discrete orientational

states are equally probable. We discretize the problem by

*dividing the tilt ( ) coordinate space into N equidistant *
intervals.

The discrete form of Eq. (7) is then obtained by rewriting the

derivatives in terms of differences18.

𝑴̇ = 𝑖𝛀 −_{𝑇} 𝐈 +_{𝜏}𝐊 ∙ 𝑴 = 𝓚 ∙ 𝑴 . (9)

𝓚 = (𝑖𝛀 − − _{𝐈 + 𝜏}− _{𝐊) represents the magnetization }

exchange matrix in inverse second units (s− ). 𝛀 is the

diagonal matrix of magnetization precession frequencies,

Ω = 𝜔±_{, }_{𝐈 the identity matrix, and 𝐊 the dimensionless }

population exchange matrix18.

The nominal exchange time is given by 𝜏 = ∆ /𝜔_{𝐷}. The

initial equilibrium magnetization equals

𝑴 = , , ⋯ , , / . (10)

This is so since the magnetization states are parametrized by

the isoprobability variable and are therefore equally

probable in the equilibrium. The formal solution to equation (9) is in terms of matrix exponent of magnetization exchange

matrix 𝓚:

𝑴 = e p(𝓚 ) ∙ 𝑴 . (11)

**Generalized dimensionless population exchange matrix. In **

the eak- ollisio li it the e ha ge o l takes pla e

between two neighbouring sites (∆ = ), equivalently 𝐊 is

tridiagonal. With the above model, , the st o g- ollisio

case, the exchange is effective between a general pair of states

( ≤ ∆ ≤ − ), can as well be addressed, by solely

generalizing the exchange matrix to include more distant off-diagonal terms, provided that it satisfies the principle of

detailed balance26. In our specific case of homogeneous

equilibrium (stationary) state (Eq. (10)), this requires that the
**sum of all elements in any row or column vanishes. **

**Relaxation dynamics of the orientational order parameter. As **

discussed above, any dynamic reorientation of nematic director, with characteristic time of the order of or shorter than the inverse rigid lattice line width, should result in the motional narrowing of the spectra. Let us now relate this

reorientational process with the exchange modelling

presented above. We conjure that at time = , the system is

ideally ordered, , = = 𝛿 − + 𝛿 + / , and

relaxes in the course of time towards the stationary

distribution, , → ∞ → _{stat} , 𝜎 (relation (4)). Within

the discrete exchange model, introduced above, this is equivalent to the initial probability vector

𝑷 = , , , ⋯ , , / , (12)

subject to exchange dynamics

𝑷̇ ̃ = 𝐊 ∙ 𝑷 (13)

solving to

𝑷 ̃ = ( ̃ , ̃ , ⋯ , − ̃ , ̃ ) = e p(𝐊 ̃) ∙ 𝑷 .

(14)

We have introduced dimensionless time ̃ = /𝜏 as the relative

time with respect to the nominal exchange time 𝜏. According

to solution (14), there exist characteristic dimensionless

times 𝜏̃ of the exchange process, corresponding to negative

inverse values of the dimensionless eigenvalues of the

population exchange matrix, 𝜏̃ = −𝜅− . In a system modelled

with a general exchange matrix 𝐊 and large number of sites ,

these times span a broad range from short ones of the order of 1 towards very large values. The stationary state

𝑷stat= 𝑷 ̃ → ∞ = , , ⋯ , , / (15)

is associated with diverging characteristic time, equivalently

with 𝜅 = that solves 𝑷̇ ̃ = 𝐊 ∙ 𝑷 _{a} = .

It is rather tedious to quantify the reorientational exchange by a spectrum of relaxation times. We simplify the description by regarding this process in terms of the associated decay of the orientational order parameter

= ∫_{−} − , , (16)

expressed in the framework of chemical exchange among nematic director orientational states as

̃ = ∑̃ ̃𝑗 ̃ ( 𝑐𝑜 𝑗− )

= (17)

Specifically, the evolution of 𝑷 ̃ from 𝑷 to 𝑷_{stat} is

associated with the evolution of ̃ from the initial ideal

order ̃ = = towards ̃ → ∞ → _{stat}. Note that the

sum in Eq. (17) is performed over ′ discrete sites with

probabilities ′ ̃ in the space of variable , whereas the

probabilities ̃ of relation (14) are calculated in discrete

points of isoprobability variable , typically with numerical

methods. In order to calculate ̃ using definition (17), one

must transform vector 𝑷 ̃ into 𝑷′ ̃ by assigning points

to equidistant points via the relation , 𝜎 , the latter

being the inverse function of , 𝜎 (Eq. (8)). ∆ must be set

to a small enough value (equivalently high enough ′ must be

chosen) so that the calculation accuracy is retained with the

above transformation. In particular, for small 𝜎 of

well-aligned samples, this implies ′ .

The decay in ̃ is inherently multi-exponential ( different

characteristic times within the discrete chemical exchange approximation, see above), and can be expressed as

The decay function ̃ is monotonously decreasing with time

from the initial value ̃ = = to ̃ → ∞ = .

We now introduce the dimensionless nominal -decay time

𝜏̃ = 𝜏 /𝜏 as the time during which ̃ decreases to 1/2:

(𝜏̃ ) − stat= − stat / ⇒ 𝜏̃ 𝜎 , , Δ . (19)

As both ̃ and _{stat} depend on 𝜎 , , and ∆ , so does

𝜏̃ = /𝜏. A representative ̃ decay is shown in Fig. 2.

**Figure 2. Time dependence of the dynamic orientational order parameter **

̃ in a partially-aligned sample with 𝜎 = ° (𝜎 = . 8). The point that
determines the nominal -decay time is marked with the orange dot. Points
in red colour were calculated using Eqs. (14) and (17) with _{=} and
∆ = . Blue solid line is an interpolated guide to the eyes.

It is noteworthy that, in the limit of large and ∆ = (weak

collision), the reorientational exchange model, introduced above, readily reproduces conventional diffusion with a

Gaussian , ̃ propagator profile

𝐺 , ̃ =_{√ 𝜋σ ̃} −

−
σ ̃ _{+} −

+

σ ̃ _{, } _{(20) }

with 𝜎 ̃ = 𝜔̃_{𝐷} ̃ = 8⁄ ̃, characteristic for a 𝐷 diffusion

process. The definition range of the tilt variable is [− , ],

so that the Gaussian approximation is only valid for 𝜎 ̃ ,

equivalently ̃ /8, since in this case the distribution does

not yet extend considerably towards = (no overlap of the

positive and negative branches of the distribution (20)). For

larger ̃, the profile of , ̃ becomes non-Gaussian and the

relation 𝜎 ̃ / 8 ̃ = is not satisfied anymore.

In the case of Gaussian propagator approximation, the dynamic order parameter can be expressed as

̃ ≈ − √_{𝜋}𝜎 ̃ + 𝜎 ̃. (21)

Evidently, condition 𝜎 ̃ that implies Gaussian profile of

, ̃ is equivalent to condition − ̃ .

**Motional narrowing of deuteron NMR spectral lines. **

**Deuteron NMR spectrum is calculated as a Fourier transform **

𝒥 𝜔 ∝ Re{∫ ℳ∞ e−iω

−∞ } (22)

of the time-dependent transversal magnetization ℳ =

∑ = . are the components of the magnetization

vector 𝑴 . By combining expressions (10) and (11) one

obtains
ℳ ∝ 𝑴T _{∙ e p(𝓚 ) ∙ 𝑴} _{ (23) }
and consequently17
𝒥 𝜈 ∝ Re{𝑴T _{[}
𝜏𝐊 − 𝜋 ℎ ho 𝐈 ± 𝑖(𝛀 − 𝜔𝐈)]
−
𝑴 }
(24)

using ℎ _{ho} = 𝜋 − and 𝜔 = 𝜋𝜈. We note again that

± stands for the two components of the deuteron quadrupole perturbed NMR doublet.

We now relate the spectrum to the relaxation dynamics of the

order parameter. The nominal exchange time 𝜏 , which

determines the nematic director reorientational exchange effectiveness, is related to the nominal -decay time via

𝜏 𝜎 , , ∆ = 𝜏𝑄

𝜏̃𝑄𝜎 , ,∆ . (25)

One can regard *Q* as the nominal time characterizing the loss

of correlations among orientational states of the nematic director, without knowing the details on the reorientational processes. With a specific choice of orientational distribution

(parameter 𝜎 ) and exchange topology (matrix 𝐊 , ∆ ),

relation (25) provides for scaling of the nominal exchange rate

𝜏− _{ with respect to }_{𝜎 , , and ∆ to value 𝜏 𝜎 , , ∆ that }

will result in a desirable Q. The dimensionless scaling

denominator 𝜏̃ 𝜎 , , ∆ is determined by methodology

described in previous subsection.

𝜏 , measured against the rigid lattice line width, is found to determine to what extent the detected spectrum will be motionally averaged. To quantify this, we introduce the

otio al a o i g effe ti e ess pa a ete

= 𝜏 Δ𝜔.l. − , (26)

with Δ𝜔_{.l.}= 𝜋Δ𝜈_{.l.} where Δ𝜈_{.l.} denotes the rigid lattice line

width. represents the rigid lattice regime, ≈ the

intermediate regime, and the strong motional

narrowing regime. 𝒥 𝜈 can then be rewritten in terms of as

𝒥 𝜈 ∝ Re{𝑴T _{[ 𝜏̃ 𝜋Δ𝜈}

.l. 𝐊 − 𝜋 ℎ ho 𝐈 ±

𝑖(𝛀 − 𝜔𝐈)]− 𝑴 }. (27)

According to above relation, if one knows the rigid lattice line

width Δ𝜈_{.l.} as well as 𝜏̃ 𝜎 , , ∆ and 𝐊 , ∆ , motional

narrowing effects can be reproduced by varying a single

parameter in the range [ , ∞] . The usefulness of the

-parametrization is in particular supported by the fact that the intermediate motional narrowing regime is reached at ≈ universally for any exchange type, i.e. independently

from 𝜎 , , and ∆ .

**Comparison of simulated and experimental deuteron NMR **
**spectra. Network component-resolved orientational order of **

structurally equivalent LCE films was determined by studying

temperature dependences of the 2H NMR spectra across the

paranematic–nematic phase transition of monodomain LCEs,

2

H-labelled on either mesogen or crosslinker molecule (Fig. 3 (b),(d)). LCEs are inherently multicomponent systems, so that differences in orientational self-organization necessarily occur even between the mesogen and the crosslinker. This is apparently the case in our LCE networks: at the transition from

the high-temperature paranematic phase into

significantly stronger orientational disorder than the mesogen (Fig. 3 (b,d)). We relate the stronger orientational disorder to the fact that molecules of crosslinker are connected by both ends to the polymer chain. Consequently, they are geometrically more confined and exhibit slower overall reorientational dynamics as compared to the mesogen molecules, attached to the backbone at one end only. The result of a slower crosslinker dynamics and therefore less averaging of the spectral lines are broader spectral features and lower spectral resolution when compared to mesogen molecules. Faster director reorientational dynamics could therefore lead to a stronger motional narrowing of mesogen spectral lines compared to crosslinker spectral lines, rendering the spectra of mesogen only seemingly less inhomogeneously broadened. Within this refined scenario, mesogens and crosslinkers might exhibit similar and rather substantial director orientational disorder.

In order to resolve the above ambiguity, a selection of
simulated spectra, calculated with reorientational exchange
model and the corresponding experimentally determined
spectra of monodomain LCEs are compared on Fig 3.
*Parameter N was set to N=100 and N= 3 in order to obtain a *
sufficiently high resolution. The simulated spectra were
generated by adjusting three parameters: the motional

narrowing effectiveness parameter , the director

orientational disorder parameter 𝜎 , and the nematic order

*parameter . fwhmhom was determined from T2* relaxation

measurements. For deuterated aromatic rings, is related to

the deuteron quadrupole perturbed NMR doublet splitting *q*

(evaluated as the difference between two Lorenzian peaks,

fitted to the experimental spectra) as follows15:

∆𝜈𝑞= 𝜈 [ − 𝑖 −_{6} +_{6}+ 𝑖 **] **

(28)

Here 𝜈 = 8 𝑘𝐻𝑧 and = . are the quadrupolar

coupling constant and asymmetry parameter, respectively, and defines the angle between the CD bond and para axis of deuteron-labelled phenyl ring of crosslinker (fixed to about 6 ° .

(a) (b) (c) (d)

**Figure 3. Series of **2H NMR spectra, calculated from the reorientational
exchange model of the nematic director (panel (a, c)) and recorded from the
paranematic to the nematic phases on a monodomain LSCE sample with 2H
phenyl ring-labelled mesogen M4 (panel (b)) and crosslinker V1 (panel (d)).
The respective temperature dependences of the simulation parameters are
shown in Fig. 4.

The estimated temperature dependences of the simulation

parameters 𝜎 and are presented in Fig. 4 for the two LSCE

samples with crosslinker V1 and mesogen M4 deuteration

sites, respectively. Similar behaviour of 𝜎 is detected in

both cases (Fig 4 (a)). At low temperatures, in the temperature

interval between 300 K and 320 K, 𝜎 monotonously increases

and matches within the experimental error for both samples. At temperatures around 330 K a weak anomaly is observed,

attributed to the nematic-smectic A transition27,28. At

temperatures above 350 K, on approaching the

paranematic-nematic transition, 𝜎 exhibits a substantial

increase, particularly in the deuterated mesogen LCE sample. We note that points above 350 K suffer from a large

experimental error, both 𝜎 and .

(a) (b)

**Figure 4. (a) Domain director alignment parameter ** and (b) motional
narrowing effectiveness parameter as a function of temperature of
the two components of the LSCE network: V1 crosslinker molecules
(green circles) and M4 mesogen molecules (red circles).

Fig. 4, panel (b) reveals monotonous increase of the motional

narrowing effectiveness parameter with increasing

temperature for both types of molecules, demonstrating that reorientational correlation times decrease with temperature and consequently result in a more effective motional

narrowing. However, in contrast to 𝜎 , is detected to

be systematically lower for the crosslinker than for the esoge , i di ati e of slo e ossli ke ’s eo ie tatio al

dynamics. This observation is also compatible with the T2

magnetization relaxation results (see section Director
**reorientation mechanism and domain misalignment) and thus **
in further support of scenario in which movement of the
crosslinker molecules is more obstructed, since these are
attached to the polymer backbone at both ends, compared
with the single side only attachment of mesogen molecules.

**Conclusions **

Differences in the temperature behaviour of orientational ordering of structurally equivalent LCEs, with almost identical mesogen/crosslinker compositions, but different deuteration

site, have been studied by 2H NMR. 2H NMR measurements

slower overall reorientational dynamics as compared with mesogen molecules, due to their geometrical restrictions originating from stronger attachment to the polymer backbone (both ends for the crosslinker vs. single end for the mesogen). The result of a slower crosslinker dynamics are also broader and more pronounced inhomogeneous spectral features. The i flue e of e ati di e to ’s o ie tatio al diso de a d

of its reorientational diffusion on the 2H NMR spectra can be

described by a simple model of director reorientational exchange, quantified by only two parameters: the static

orientational disorder parameter 𝜎 and the nominal

orientational order decay time 𝜏 . Comparative analysis of

theoretically modelled and experimentally determined

deuteron NMR spectra reveals that both crosslinker and

mesogen molecules exhibit similar, substantial static

orientational disorder. The disorder is lower at room temperature and monotonously increases on approaching the paranematic nematic transition at about 350 K. The quantitatively similar orientational disorder, detected for the

crosslinker and mesogen molecules, is in apparent

contradiction with experimentally detected substantially higher inhomogeneous broadening of the crosslinker deuteron spectrum as compared to the mesogen spectrum. Somewhat surprisingly, our results support the scenario of similar degree of orientational disorder, by attributing the mismatch in spectral shapes to faster reorientational dynamics of mesogens, (vs. crosslinker), as identified through much higher value of the motional narrowing effectiveness parameter.

** References **

*1 M. Warner and E. M. Terentjev, Liquid Crystal Elastomers, *
International Series of Monographs on Physics 120, 2003.
*2 W. H. de Jeu, Ed., Liquid Crystal Elastomers: Materials and *

*Applications, Springer Berlin Heidelberg, Berlin, Heidelberg, *

2012, vol. 250.

**3 E. M. Terentjev, J. Phys. Condens. Matter, 1999, 11, R239. **

* 4 V. Domenici, Prog. Nucl. Magn. Reson. Spectrosc., 2012, 63, 1*–

32.

5 *J. Küpfe a d H. Fi kel a , Makromol. Chem. Rapid Commun., *

**1991, 12, 717–726. **

* 6 K. A. Burke and P. T. Mather, J. Mater. Chem., 2010, 20, 3449*–

3457.

7 V. Do e i i, G. A ožič, M. Čopič, A. Le a , I. D e e

*šek-Ole ik, P. U ek, B. Zala , B. Zupa čič a d M. Žigo , Polymer, *

**2009, 50, 4837**–4844.

**8 H. Jiang, C. Li and X. Huang, Nanoscale, 2013, 5, 5225–5240. ***9 M.-H. Li and P. Keller, Philos. Trans. R. Soc. Math. Phys. Eng. Sci., *

**2006, 364, 2763–2777. **

10 M. Camacho-Lopez, H. Finkelmann, P. Palffy-Muhoray and M.

* Shelley, Nat. Mater., 2004, 3, 307*–310.

11 F. G e o, V. Do e i i, S. Ro iti, T. Assaf, B. Zupa čič, J. Mila e ,

*B. Zalar, B. Mazzolai and V. Mattoli, Mol. Cryst. Liq. Cryst., 2013, *

**572, 40**–49.

*12 G. Abbandonato, D. Catalano, V. Domenici and B. Zalar, Liq. *

* Cryst., 2012, 39, 165*–174.

13 V. Do e i i, J. Mila e , B. Zupa čič, A. Bu o , V. Ha plo a

* and B. Zalar, Magn. Reson. Chem., 2014, 52, 649*–655.

*14 G. Feio, J. L. Figueirinhas, A. R. Tajbakhsh and E. M. Terentjev, J. *

**Chem. Phys., 2009, 131, 074903. **

* 15 V. Domenici and B. Zalar, Phase Transit., 2010, 83, 1014*–1025.

16 P. J. Se astião, D. Sousa, A. C. Ri ei o, M. Vilfa , G. Lahaj a , J.

**Selige a d S. Žu e , Phys. Rev. E, 2005, 72, 061702. ***17 A. Abragam, The principles of nuclear magnetism., Clarendon *

Press, Oxford, 1961.

*18 B. Zalar, R. Blinc, S. Zumer, T. Jin and D. Finotello, Phys. Rev. E *

**Stat. Nonlin. Soft Matter Phys., 2002, 65, 041703. **

*19 A. Lebar and B. Zalar, NMR investigation of monodomain liquid *

*crystal elastomer: doctoral thesis, [A. Lebar], Ljubljana, 2006. *

*20 B. Cowan, Nuclear Magnetic Resonance and Relaxation, *
Cambridge University Press, Cambridge; New York, 2005.
*21 V. Domenici, M. Geppi and C. A. Veracini, Prog. Nucl. Magn. *

* Reson. Spectrosc., 2007, 50, 1*–50.

* 22 Z. Luz and S. Meiboom, J. Chem. Phys., 1963, 39, 366–370. *
23 V. Domenici, J. Milavec, A. Bubnov, D. Pociecha, B. Zupancic, A.

*Resetic, V. Hamplova, E. Gorecka and B. Zalar, RSC Adv., 2014. *
*24 S`achez Ferrer Antoni, Photo-active liquid crystalline elastomers: *

*doctoral thesis, Barcelona, vol. 2006. *

*25 C. P. Slichter, Principles of Magnetic Resonance, Springer, *
Be li ; Ne Yo k, 3 d e la ged a d updated ed. 99 . Co . 3 d
printing 1996 edition., 1996.

* 26 M. J. Klein, Phys. Rev., 1955, 97, 1446*–1447.

27 D. M. Lambreva, B. I. Ostrovskii, H. Finkelmann and W. H. de
**Jeu, Phys. Rev. Lett., 2004, 93, 185702. **

28 W. H. de Jeu, B. I. Ostrovskii, D. Kramer and H. Finkelmann,